Dynamic Coating Using Polyelectrolyte Multilayers for Chemical Control of Electroosmotic Flow in Capillary Electrophoresis Microchips. Yan Liu, Joseph C.
Jun 19, 2013 - layer-by-layer (LbL) sequential deposition followed by cross- ... KEYWORDS: marine fouling, polyelectrolyte, layer by layer assembly, covalent ...
Jun 19, 2013 - XPS data processing, including peak assignment and peak fitting (fitting algorithm Simplex), was done using the software package Thermo Avantage, version 4.12 (Thermo Fisher .... The high control over the thickness of films, constructe
Sep 29, 2014 - Department of Physics, Ulsan National Institute of Science and Technology (UNIST), Ulsan 689-798, Korea. Â§. Department of Chemistry ...
May 14, 2008 - E-mail: [email protected], â ... Matthew A. Caporizzo , Carlo A. Daep , David M. Eckmann , James G. Masters , and Russell J. Composto.
Jun 24, 2003 - UniteÂ´ de Chimie des MateÂ´riaux Inorganiques et Organiques, ... Place L. Pasteur, 1, B-1348 Louvain-la-Neuve, Belgium (European Union).
Sep 29, 2014 - Molybdenum disulfide (MoS2) multilayers with functional polyelectrolyte nanospacing layers are presented. Taking advantage of the facile method of layer-by-layer (LbL) assembly, individual chemically exfoliated MoS2 layers are not only
Selective Electroless Nickel Plating on Polyelectrolyte Multilayer Platforms ..... TrAC Trends in Analytical Chemistry 2010 29 (8), 870-884 .... Networks of ChargeâCharge Interactions in Proteins Measured by Charge Ladders and .... with additional
Subscriber access provided by McMaster University Library
Water Sorption in MXene/Polyelectrolyte Multilayers for Ultrafast Humidity Sensing Hyosung An, Touseef Habib, Smit A. Shah, Huili Gao, Anish Patel, Ian Echols, Xiaofei Zhao, Miladin Radovic, Micah J. Green, and Jodie L. Lutkenhaus ACS Appl. Nano Mater., Just Accepted Manuscript • DOI: 10.1021/acsanm.8b02265 • Publication Date (Web): 03 Jan 2019 Downloaded from http://pubs.acs.org on January 6, 2019
Just Accepted “Just Accepted” manuscripts have been peer-reviewed and accepted for publication. They are posted online prior to technical editing, formatting for publication and author proofing. The American Chemical Society provides “Just Accepted” as a service to the research community to expedite the dissemination of scientific material as soon as possible after acceptance. “Just Accepted” manuscripts appear in full in PDF format accompanied by an HTML abstract. “Just Accepted” manuscripts have been fully peer reviewed, but should not be considered the official version of record. They are citable by the Digital Object Identifier (DOI®). “Just Accepted” is an optional service offered to authors. Therefore, the “Just Accepted” Web site may not include all articles that will be published in the journal. After a manuscript is technically edited and formatted, it will be removed from the “Just Accepted” Web site and published as an ASAP article. Note that technical editing may introduce minor changes to the manuscript text and/or graphics which could affect content, and all legal disclaimers and ethical guidelines that apply to the journal pertain. ACS cannot be held responsible for errors or consequences arising from the use of information contained in these “Just Accepted” manuscripts.
Water Sorption in MXene/Polyelectrolyte Multilayers for Ultrafast Humidity Sensing Hyosung An,1 Touseef Habib,1 Smit Shah,1 Huili Gao,2 Anish Patel,1 Ian Echols,1 Xiaofei Zhao,1 Miladin Radovic,2,3* Micah J. Green,1,3* and Jodie L. Lutkenhaus1,3* 1Artie
McFerrin Department of Chemical Engineering, Texas A&M
University, College Station, Texas 77843, USA. 2Department
of Mechanical Engineering, Texas A&M University,
College Station, Texas 77843, USA. 3Department
of Materials Science and Engineering, Texas A&M
University, College Station, Texas 77843, USA.
KEYWORDS. MXene, Titanium carbides, Layer-by-layer assemblies, Water sorption, Humidity sensors.
noninvasive epidermal sensing, and environmental monitoring bring forward the need for fast humidity sensors. However, achieving a rapid response to dynamic changes in humidity, such as for human respiration, is challenging. This is because the response can be limited by the diffusion of water, the sorption of water in the material, and the sensing method itself. Here, the water sorption and response mechanism for multilayer assemblies made from MXene nanosheets and polyelectrolytes for ultrafast humidity sensing are described. MXenes are a class of two-dimensional transition metal carbides (e.g., Ti3C2) possessing hydrophilicity and metal-like conductivity. Herein we show that MXene/polyelectrolyte multilayer films
response and recovery times exceeding those of most humidity sensors. Quartz crystal microbalance and ellipsometry support the mechanism that upon changing humidity, water molecules intercalate into (or deintercalate from) the MXene/polyelectrolyte multilayer, resulting in an increase (or a decrease) in the thickness and sheet-to-sheet distance, which then changes the tunneling resistance
demonstrated by monitoring real-time human respiration using a portable microcontroller for wireless sensing.
Humidity sensing is significant in a wide range of applications in
metallurgy, and climatology.1-12 Recently, humidity sensors with fast response have been desired for emerging technologies, such as wearable
Although there are many reported humidity sensors using optical,16, 17
and magnetoelastic25 methods, many of these
methods are still challenged by the response and recovery times. We hypothesized that two-dimensional metal carbides (referred to as MXenes, or Mn+1XnTx, where M is an early transitional metal, X is either carbon or nitrogen, and T is a surface terminal group, such as -F, -OH, -O, and -Cl) would be promising materials for humidity
conductivity (2 × 105 S/m).26 Dillon et al. demonstrated changes in sheet
nitrogen,27 and Shpigel et al. demonstrated water sorption in MXene electrodes response
response mechanism were not discussed or understood. Recently, we demonstrated highly stretchable MXene/polyelectrolyte multilayers assembled using the layer-by-layer (LbL) assembly technique as strain sensors in which resistance was correlated to in-plane tensile strain.28 We here hypothesized that MXene/polyelectrolyte
multilayers might be responsive to humidity by a mechanism where water
consequentially increases the resistance of the bulk electrode. We first prepared MXene/polyelectrolyte multilayers using LbL assembly,
polyelectrolytes each for 15 min of adsorption time (Figure 1a). Ti3C2Tx MXene sheets were derived from the parent Ti3AlC2 MAX phase29 and had a lateral sheet size of about one micrometer (Figure S1). The MXene nanosheets were negatively charged (-32 mV by zeta potential) in water at pH 5, while poly(diallyldimethylammonium chloride) (PDAC) at pH 5 was used as the complementary positively charged species (+18 mV) for assembly. As the number of layer pairs (or LbL cycles) increased from zero to five, the color of the film became visibly darker (Figure 1b), which indicated the successful assembly
immersive LbL process to yield MXene multilayers having a mixed layer structure.30-33 Note that we tried or evaluated other processing methods (i.e., casting, simple
difficult to process by spin-casting or solution-casting. Vacuum assisted filtration MXene-polymer papers have been reported.34 For example, MXene sheets were mixed with PVA or PDAC in water, and
then filtered to produce a free-standing paper; however, this technique cannot produce a thin nanometer-scale coating. However, we chose layer-by-layer assembly here because it fulfills the multiple controlled
conformal coatings even on complex surfaces, and (4) balance between multiple functional properties. We
MXene/polyelectrolyte multilayer in the early stages of growth to determine the minimum number of layer pairs needed to achieve inplane percolation. Scanning electron microscopy (SEM) confirmed dense coverage of the MXene sheets on the surface and parallel arrangement of the MXene sheets in a brick-and-mortar-like fashion, (Figure 1c and 1d). UV-vis spectra of the MXene/polyelectrolyte multilayers show a broad adsorption feature at 770 nm assigned to MXene nanosheets35,
that increased with the number of layer pairs,
(Figure 1e). Similarly, the film thickness increased linearly as 9.5 nm per layer pair (or LbL cycle), Figure 1f. Similarly, the film thickness increased linearly at 9.5 nm per layer pair (or LbL cycle), Figure 1f. With the assumption that the coated polymer thickness is negligible and that the major contribution to thickness comes from MXene sheets (the average thickness of an MXene sheet: ~1 nm),37, 38 about 9-10 layers of MXene sheets were deposited during each MXene adsorption step. The root-mean-square roughness was lower than 20 nm, as measured by profilometry (Figure 1g). These results confirm that linear growth occurs even in the
early stages of growth, and complements our early findings that show linear growth continues up to 40 layer pairs.28 Table
multilayers of two, three, and five layer pairs for which the PDAC and
multilayer had a conductivity of 21 S/cm, which increased slightly to 27 ± 2 S/cm for five-layer pairs. A two-layer-pair multilayer’s conductivity
percolation of the MXene sheets. Similar results were obtained for MXene/polyelectrolyte multilayers with reduced PDAC adsorption times of 5 and 10 min, in which the highest conductivity was 47 ± 5 S/cm for a five-layer pair multilayer with 5 min PDAC adsorption time. Based on these results, we conclude that a minimum of three layer pairs is needed to achieve in-plane percolation of MXene sheets and that reduced PDAC content enhances conductivity. We next examined how resistance changed with varying relative humidity for the MXene/polyelectrolyte multilayer for which the PDAC and MXene adsorption times were 15 min. For a patterned MXene/polyelectrolyte multilayer on PET (Figure 2a), resistance increased by 52% as relative humidity (RH) increased from 10% to 70%
decreasing the relative humidity back to 10% (Figure 2b). In addition, the MXene/polyelectrolyte
films showed a
stable resistance response over the course of 100 cycles (or 3 h)
of switching from 30% RH to 40% RH. (Figure 2c). This result indicates that the reversible resistance change is due to water adsorption, not oxidation of MXene sheets.39 As shown in Figure S2, a long-term stability test showed that sensors stored in ambient conditions
increase in resistance, indicating probable MXene oxidation.40-43 For all other experiments, we stored samples in hermetically sealed Argon-filled vials at 5˚C before any tests to prevent oxidation.43 To understand the underlying mechanism of the reversible and repeatable resistance change, we investigated water sorption and film thickness at varying relative humidity values. Measurements using
MXene/polyelectrolyte multilayers, which followed a Freundlich isotherm model44,
(Figure 2d and 2f, and analysis shown in
Supporting Information). Ellipsometry measurements also verified the
reversible and stable resistance change in Figure 2b and 2c. Shpigel et. al. reported that Ti3C2 electrodes contain 0.75 g/cm3 of water.28 A quarter of the water was trapped in the interspaces between MXene nanosheets, and three quarters was moveable water placed
MXene/polyelectrolyte multilayers had lower water sorption (0.37
g/cm3 at 70% RH) than that of the Ti3C2 electrodes reported by Shpigel et
immersed in water and our electrodes contain polyelectrolyte. Also, the reported contact angle of MXene nanosheets is 35o.34 PDAC finished (or covered) LbL films bear a contact angle of about 25o.46 The proposed humidity response mechanism is shown in Figure 3a. Upon increasing humidity, MXene interlayer distance
sheet-to-sheet distance) increases,
tunneling resistance (Figure 3b-f and analysis shown in Supporting Information). Upon lowering the humidity, the interlayer distance decreases, and the resistance recovers. A similar mechanism has been observed elsewhere for silver nanowire strain sensors and for carbon
Another possible contribution to the mechanism is a reduction in conductivity caused by interaction of a polar molecule with the MXene’s surface terminal group (-OH), thus changing the electronic structure of the MXene itself.48 Based on the studies below, it appears that the dominating mechanism is the change in interlayer spacing. To
spacing between MXene layers by adjusting the PDAC deposition time (5 min, 10 min, or 15 min) while keeping MXene deposition time at 15 min (Figure S3a to S3h). In essence, this adjusts the PDAC content, which, in turn, affects the interlayer spacing and the sheet-to-sheet tunneling resistance response. QCM confirmed that
composition increased (6.1 wt% for 5 min, 7.8 wt% for 10 min, and 9.3 wt% for 15 min, Figure 4a and S3i and Table S2). Increasing the PDAC deposition time led to an increase in the mass of PDAC deposited, which probably led to an increase in the sheet-to-sheet distance (or interlayer spacing), as suggested by changes in the X-ray diffraction (XRD) pattern (Figure S4). As shown in Table S1, the conductivity decreased with increasing PDAC deposition time (e.g., 47 S/cm and 27 S/cm for a five-layer pair multilayer with 5 min and 15 min PDAC deposition, respectively). As PDAC deposition time increased from 5 to 15 min, the sensitivity to humidity increased by 46% (comparing R/R10% at 70% RH, Figure 4b) and thickness change increased by 33% (Figure 4c). These results indicate that the humidity response is dependent on the PDAC content
resistance response. This supports our hypothesis that reversible water insertion into their interlayer gaps results in changing their interlayer distance and electrical resistance. We speculate that the response bears dual contributions from the polymer and the MXene, but these cannot be decoupled at present. The
MXene/polyelectrolyte multilayers were evaluated (Figure 4d) using an electric fan that periodically interrupted the flow of humid air at a frequency of 1/3 Hz. It should be noted that many humidity
sensors measured response time test (or recovery time test) with widely different RH ranges.13,
14, 22, 49-55
For equitable comparison,
we introduce the “time per RH range tested” (having units of sec/RH) as a figure of merit with the assumption that humidity response is linear. All three samples (with 5 min, 10 min and 15 min PDAC deposition) showed short response and recovery times of 110 ms and 220 ms, respectively, corresponding to response and recovery times per RH of 0.005 sec RH-1 and 0.01 sec RH-1, respectively. These fast response and recovery times are comparable to ultrafast humidity sensors using graphene,56 carbon nitride,22 silicon nanocrystals,14 and graphene oxide13, as well as a commercially available ultrafast sensor23 (Figure 4e and 4f and Table S313-15,
To gain insight into the kinetics of the humidity response, the rate constants were calculated as the resistance change due to water (de)sorption70-72 (Figure S5) as follows: ln((R1 – R0)/(R1 – Rt)) = ksorp t or kdesorp t, where R1 is the final resistance of the MXene/polyelectrolyte multilayers, R0 is the initial resistance, Rt is the resistance at time t, and ksorp and kdesorp are the rate constants at increasing and decreasing humidity, respectively. As the PDAC deposition time increased, ksorp decreased as 17.4 s-1, 10.2 s-1, and 9.5 s-1 for 5 min, 10 min, and 15 min PDAC deposition time, respectively. A similar result was obtained for kdesorp (7.3 s-1,
respectively). This indicates that
increased deposition time and increased PDAC content, leads to
markedly different rate constants, which indicates that PDAC plays a major role in sensing. As PDAC sorbs and desorbs water, it likely adjusts the interlayer or flake spacing and overall film thickness (indirectly evidenced in Figure 2e). The
MXene/polyelectrolyte multilayers could be used as human health sensors to monitor human respiration. For demonstration, a sensor was fabricated using a patterned MXene/polyelectrolyte multilayer on PET and an Arduino microcontroller (Figure 5a and 5b and Figure S6).
changes in humidity due to inhalation and exhalation (Figure 5c and Movie S1). Because of the rapid response time, real-time monitoring was achieved, (Figure 5d-h). The volunteer walked for 90 sec, ran for 90 sec, and then walked again. As the volunteer ran, the respiration rate increased from 15 min-1 to 23 min-1 (Figure 5e and 5f). When the volunteer walked once more, the respiration rate was 31 min-1 because the volunteer had shortened breath (Figure 5g). After a minute, their respiration renormalized (15 min-1) (Figure 5h). Similar profiles were observed in ultrafast humidity sensors using cellulose73 and silicon-nanocrystals.14 In summary, these results demonstrate that thin MXene/polyelectrolyte multilayers can detect changes in humidity with ultrafast response and recovery and excellent reversibility. This concept may be applicable to various applications in many
medical or environmental applications, where the humidity may change dynamically and rapidly. We found that MXene multilayers have tradeoffs between increased conductivity and decreased sensitivity. As conductivity decreased (e.g., 47 S/cm and 27 S/cm for a five-layer pair multilayer with 5 min and 15 min PDAC deposition, respectively), the sensitivity to humidity increased by 46% (comparing R/R10% at 70% RH, Figure S7). In contrast, as conductivity decreased, the kinetics (i.e., rate constants) of the humidity response decreased. For examples, as the PDAC deposition time increased, ksorp decreased as 17.4 s-1, 10.2 s-1, and 9.5 s-1 for 5 min, 10 min, and 15 min PDAC deposition time, respectively. These results suggest that increasing conductivity did not improve all aspects of humidity sensing properties in our system. On the other hand, Jung et al. explored the change in resistance of (pure) MXene papers in response to various gas vapors.48 They found that the MXene papers had much higher conductivity than as reported here (32.5 S/cm vs 47 S/cm, respectively) and that the high conductivity led to an exceptional sensitivity toward polar gas vapors. The present work herein has lower sensitivity because of PDAC’s insulating nature. Yet, PDAC, because it participates in the humidity sensing mechanism, has a significant and observable response toward humidity. Looking forward, the humidity response might be further modulated or amplified using highly water-sensitive polymers. The modeling of the tunnel resistance changing with MXene distance indicates that even stronger responses are possible with polymer layers that
can switch between a highly expanded coil state and collapsed state. This also points to the possibility of MXene/polymer sensors based upon changes in resistance. For example, pH- or temperatureresponsive polymers would also adjust the MXene sheet spacing, thus changing tunneling resistance.
Experimental section Materials: Poly(diallyldimethylammonium chloride) (PDAC, MW = 200,000 – 350,000 g mol-1, 20 wt% in water), hydrochloric acid (HCl, ACS reagent, 37% w/w), and dimethyl sulfoxide (DMSO, ReagentPlus, >99.5%)
particle size, 99.5% purity), Al (44 μm average particle size, 99.5% purity), TiC powders (2 – 3 μm average particle size, 99.5% purity), lithium fluoride (LiF, 98+% purity) were purchased from Alfa Aesar. Substrates for
layer-by-layer deposition included
slide glass (VWR) and PET (Melinex ST505, Tekra). Synthesis of Ti3AlC2 MAX phase: Commercial Ti, Al and TiC powders were used as starting raw materials to synthesize Ti3AlC2 MAX phase. To prepare homogeneous powder mixtures, Ti, Al and TiC powders were first weighed to achieve Ti:Al:C=3.0:1.2:1.8 ratio and mixed together using ball-milling with zirconia beads in a glass jar at the speed of 300 rpm for 24 hours. Then, the bulk high-purity Ti3AlC2 samples were sintered at temperature of 1510 °C for 15 mins with a loading of 50 MPa using a pulsed electric current system (PECS). To fabricate high-purity Ti3AlC2 powder, the PECSed sample was first drill-milled and sieved to obtain powder with particle sizes below 44 μm. Synthesis of Ti3C2Tx MXene clay: Ti3C2Tx MXene clay was synthesized by etching aluminum from the MAX phase using the technique described by Ghidiu et.al.37 Concentrated HCl (37% w/w) was diluted with deionized (DI) water to obtain 30 mL of 6 M HCl solution. This solution
was transferred to a polypropylene (PP) beaker, and 1.98 g of LiF was added to it. This dispersion was stirred for 5 minutes using a Teflon (PTFE) magnetic stirrer at room temperature. Ti3AlC2 MAX phase powder was slowly added to the HCl+LiF solution to prevent overheating as the reaction is highly exothermic. The PP beaker was capped to prevent evaporation of water and a hole was made in the cap to avoid buildup of gases. The reaction mixture was stirred at 40 ºC for about 45 hours. The slurry product was filtered and washed with DI water in a polyvinyl-difluoride (PVDF) filtration unit with pore size of 0.22 µm (Millipore® SCGVU10RE Stericup™ GV) to remove the unreacted HF and water-soluble salts. This washing process was repeated until the pH of the filtrate reached a value of about 6. Reaction product collected over the PVDF filter was extracted as Ti3C2Tx MXene clay. Intercalation and delamination of Ti3C2Tx MXene clay: Ti3C2Tx MXene clay was intercalated with DMSO and subsequently bath sonicated to obtain a dispersion of delaminated Ti3C2Tx MXenes. DMSO was added to Ti3C2Tx MXene clay (dried in vacuum oven for about 24 hours at 40 °C) to form a 60 mg ml-1 suspension followed by about 18 hours of stirring at room temperature. After intercalation, excess DMSO was removed by several cycles of washing with DI water and centrifugation at 5000 rpm for 4 hours. The intercalated Ti3C2Tx MXene suspension in DI water was bath sonicated for 1 hr at room temperature followed by centrifugation at 3500 rpm for 1 hour to separate the heavier components. The supernatant contained the stable Ti3C2Tx nanosheet dispersion. Preparation of MXene/polyelectrolyte multilayers: The PDAC and MXene sheets were diluted to a concentration of 1.0 mg ml-1 in deionized water (18.2 MΩ). The pH values of the PDAC solution and MXene dispersion were 5.0 and 5.0, respectively, and both solutions were used without adjusting the pH. For layer-by-layer deposition
onto pure PET, a PET sheet was cut into 12.5 mm × 50 mm and then cleaned with isopropyl alcohol and water. After washing, the PET was dried with nitrogen. To make a U-shaped pattern, 1 mm wide tape was placed on PET substrate prior to layer-by-layer assembly. Plasma treatment (Harrick PDC-32G) was conducted for 5 min. Plasma treated PET substrates were immersed in PDAC solution for 15 min, and rinsed with deionized water for 2, 1, and 1 min each. Then, the substrates were immersed in MXene dispersion for 15 min, and rinsed with deionized water for 2, 1, and 1 min each. The same procedure was repeated until the desired thickness was obtained. To prepare the MXene/polyelectrolyte multilayers with different PDAC, we have varied PDAC deposition time (5 min, 10 min, and 15 min) while keeping MXene deposition time for 15 min. Each cycle is termed as a “layer pair”, After layer-by-layer coating, the films were cut into 3.13 mm × 50 mm and then the tape was removed. Copper wires were connected to both ends of the U-shaped patterned layerby-layer film (Fig. 2a) using silver paste followed by drying under vacuum for 4 hr. For humidity sensing, the copper wires of the sensors were connected to a multimeter. Characterization: Scanning electron microscopy (SEM, JEOL JSM7500F) was used to investigate morphologies of the multilayer films. 3 nm of platinum/palladium alloy was sputter-coated onto samples prior to imaging. Profilometry (P-6, KLA-Tencor) was used to measure the thickness of the MXene-based multilayer in at least
five different locations. A manual four-point resistivity probe (Lucas
conductivity of the multilayer. UV-vis spectroscopy was conducted using a Shimadzu UV-2401 PC spectrometer over a wavelength range of 300-900 nm. Ellipsometry (Gaertner LSE Stokes ellipsometer) was used to measure the thickness of MXene/polyelectrolyte multilayers on silicon substrate. The mass composition of the multilayer was measured using quartz crystal microbalance (QCM) (Inficon, Maxtek RQCM). First, plasma treatment (Harrick PDC32G) was carried out on a 5 MHz Ti/Au quartz crystal for 5 min. The multilayer was deposited assembly
multilayer was determined by monitoring the frequency changes during each layer deposition from 0 to 5 layer pairs. Mass was calculated
equation.74 The humidity response of the MXene/polyelectrolyte multilayer was measured in a homebuilt chamber. All sensing experiments were conducted
bubbling dry air (~0% RH) in distilled water. Relative humidity in the box was simultaneously recorded using a commercial humidity sensor (Willhi WH1436H). The accuracy of the commercial sensor was ±1%. The resistance of the MXene film during the humidity test was measured using a multimeter (Peakmeter PM8236 Digital Multimeter).
Ellipsometry and QCM were used to measure the film thickness and mass, respectively, as a function of humidity. As for evaluation of response and recovery time, flowing humid air was modulated by passing it through a home-built electric fan using an Arduino Uno R3 (Elegoo) and a stepper motor (Elegoo 28BYJ-48). The RH range for the response and recovery time tests was 20 to 40% RH. For the long-term stability test, we stored MXene multilayer samples in ambient conditions and conducted humidity sensing as a function of time. As for real-time monitoring of human respiration, the sensor was originally under ambient conditions with relative humidity around 25%. The resistance of the sensor was recorded using an Arduino Uno R3. Note that direct contact with PDAC may be harmful and cause skin irritation.
Figure 1. Characterization of MXene/polyelectrolyte multilayers assembled using LbL technique. (a) Schematic of the PDAC/MXene assembly. (b) A digital image of MXene/polyelectrolyte multilayer films of varying layer pair numbers (0, 2, 3, and 5) on glass, prepared by the sequential adsorption of PDAC and MXene for 15 min each. (c) A top-down and (d) a cross-sectional SEM image of MXene/polyelectrolyte multilayer films (10 layer pairs). (e) UVvis absorption spectra of the MXene/polyelectrolyte multilayer films. An inset image shows absorbance values at 770 nm versus number
Figure 2. Humidity sensing properties for MXene/polyelectrolyte multilayers
MXene/polyelectrolyte multilayer film on PET with copper wire connections. (b)
Normalized resistance (R/R10%) versus wet-dry
cycles for multiple humidity values ranging from 10% RH to 70% RH. (c) Cycling performance alternating between 30% RH and 40% RH at room
ellipsometric thickness change to demonstrate water sorption into the MXene/polyelectrolyte multilayers at various relative humidity values. (f) Adsorption isotherms of water for a 5-layer-pair MXene/polyelectrolyte multilayer at 294 K normalized against the
film mass at 10% RH. The Freundlich isotherm equation is described as follows: ln (Δm/m10%) = ln Kf + ln (RH)/n where m10% is the MXene/polyelectrolyte multilayer mass at 10% RH, Δm is the absorbed water mass, Kf is a Freundlich affinity coefficient, RH is relative humidity (the ratio of the partial pressure of water vapor to the equilibrium vapor pressure of water a given temperature), and n is a dimensionless number.
multilayers and the corresponding electrical circuit models for (b, c) low and (d, e) high humidity, which explain electrical interconnections of three adjacent MXenes (dark gray in Figure 3b and 3d). R1, R2, and R3 are MXene nanosheet resistance and Rt1 and Rt2 are tunneling resistances at the junctions. (f) Response of the multilayer to the varying relative humidity by experimental measurements and numerical modelling (for a detailed analysis, see Supporting Information).
Figure 4. Humidity sensing behavior of the MXene/polyelectrolyte multilayer films processed with different PDAC deposition times of 5 min, 10 min, and 15 min. (a) MXene/polyelectrolyte multilayer film composition. (b) Normalized resistance and (c) thickness
versus wet-dry cycles, where the percentages are the relative humidity
MXene/polyelectrolyte multilayers with different PDAC deposition times. The dashed lines indicate the response and recovery times. (e-f)
humidity sensors reported in the literature, where the recovery and response times are normalized by the relative humidity interval investigated. Figure 4f shows the dashed box in Figure 4e. See Table S3 for references.
ASSOCIATED CONTENT Supporting Information. The following files are available free of charge. An AFM image of single MXene flake, a long-term stability test, Freundlich isotherm model, modeling the resistance change, characteristics of MXene/polyelectrolyte multilayers with varying PDAC deposition time, XRD data, calculation of rate constants (ksorp or kdesorp), digital images of wireless humidity sensors, characteristics of reported humidity sensors (PDF) A demonstration of a MXene/polyelectrolyte multilayer film integrated with an Arduino microcontroller monitoring human respiration in real-time (MOV)
H.A. and A.P. prepared and characterized the MXene multilayers with supervision by J.L.L. T.H and S.S. synthesized and characterized the MXene nanosheets with supervision by M.J.G. H.G. prepared the MAX phases with supervision by M.R. J.L.L. claims responsibility for all the figures in the main text and the Supplementary Materials. All authors completed the data analysis and prepared the manuscript. Funding Sources This material is based upon work supported by the National Science Foundation under Grant No. 1760859. ACKNOWLEDGMENT This material is based in part upon work supported by the National Science
Kwanjeong Educational Foundation and Texas A&M Energy Institute for financial support.
Oxide-Silicon Bi-Layer Flexible Structure. Sensors and Actuators B: Chemical 2012, 161 (1), 1053-1058. 24.
Xu, J.; Bertke, M.; Li, X.; Yu, F.; Hamdana, G.; Peiner, E., Fabrication of ZnO Nanorods
and [email protected] ZnO Nanorods on MEMS Piezoresistive Self-Actuating Silicon Microcantilever for Humidity Sensing. Sensors and Actuators B: Chemical 2018. 25.
Grimes, C. A.; Kouzoudis, D.; Dickey, E. C.; Qian, D.; Anderson, M. A.; Shahidain, R.;
Lindsey, M.; Green, L., Magnetoelastic Sensors in Combination with Nanometer-Scale Honeycombed Thin Film Ceramic TiO2 for Remote Query Measurement of Humidity. Journal of Applied Physics 2000, 87 (9), 5341-5343. 26.
Surface Structure and Intercalation Mechanism of Ti3C2X. Journal of the American Chemical Society 2015, 137 (7), 2715-2721. 39.
Römer, F. M.; Wiedwald, U.; Strusch, T.; Halim, J.; Mayerberger, E.; Barsoum, M. W.;
Farle, M., Controlling the Conductivity of Ti3C2 MXenes by Inductively Coupled Oxygen and Hydrogen Plasma Treatment and Humidity. RSC Advances 2017, 7 (22), 13097-13103. 40.
Ghassemi, H.; Harlow, W.; Mashtalir, O.; Beidaghi, M.; Lukatskaya, M.; Gogotsi, Y.;
Taheri, M. L., In Situ Environmental Transmission Electron Microscopy Study of Oxidation of Two-Dimensional Ti3C2 and Formation of Carbon-Supported TiO2. Journal of Materials Chemistry A 2014, 2 (35), 14339-14343. 41.
Halim, J.; Cook, K. M.; Naguib, M.; Eklund, P.; Gogotsi, Y.; Rosen, J.; Barsoum, M. W.,
X-Ray Photoelectron Spectroscopy of Select Multi-Layered Transition Metal Carbides (MXenes). Applied Surface Science 2016, 362, 406-417.